Post on 14-Apr-2016
Embed Size (px)
DESCRIPTIONPolymer Matrix composite with nanoparticle reinforcement
Materials 2010, 3, 3468-3517; doi:10.3390/ma3063468
materials ISSN 1996-1944
Polymer-Nanoparticle Composites: From Synthesis to Modern Applications
Thomas Hanemann 1,2,* and Dorothe Vinga Szab 1
1 Institute for Materials Research, Karlsruhe Institute of Technology (KIT), Hermann-von-Helmholtz-Platz 1, D-76344 Eggenstein-Leopoldshafen, Germany; E-Mail: firstname.lastname@example.org (D.V.S.)
2 Institute for Microsystems Engineering (IMTEK), University of Freiburg, Georges-Koehler-Allee 102, D-79110 Freiburg, Germany
* Author to whom correspondence should be addressed; E-Mails: email@example.com or firstname.lastname@example.org; Tel.: +49-7247-82-2585; Fax: +49-7247-82-2095.
Received: 23 April 2010 / Accepted: 27 May 2010 / Published: 28 May 2010
Abstract: The addition of inorganic spherical nanoparticles to polymers allows the modification of the polymers physical properties as well as the implementation of new features in the polymer matrix. This review article covers considerations on special features of inorganic nanoparticles, the most important synthesis methods for ceramic nanoparticles and nanocomposites, nanoparticle surface modification, and composite formation, including drawbacks. Classical nanocomposite properties, as thermomechanical, dielectric, conductive, magnetic, as well as optical properties, will be summarized. Finally, typical existing and potential applications will be shown with the focus on new and innovative applications, like in energy storage systems.
Keywords: nanocomposites; polymer matrix; spherical nanoparticles; physical property tailoring, polymer-nanoparticle-interface
Materials 2010, 3
Within the last 15 years, materials and structures showing geometric dimensions below 100 nm have gained more and more attraction to the scientific world and stimulated spirit of research on sometimes fancy ideas for future applications like molecular manufacturing or space elevators as well as on serious products for consumer goods, health, medical or food technology [1-5]. With respect to the almost infinite numbers of scientific reports, books, and journal contributions on nanoscience and nanotechnology, the authors of this review article concentrate on some elementary considerations on inorganic nanoparticle properties, basic remarks on synthesis and processing challenges, functional properties and applications of polymer-nanoparticle-composites, as well as on modern research fields, where these polymer matrix composites play a decisive role:
optical and magnetic properties microelectronic devices piezoelectric actuators and sensors electrolytes, anodes in lithium-ion-batteries and supercapacitors organic solar cells and intrinsic conductive polymers photoresists used in microelectronics and microsystems technologies biomedical sciences.
Before discussing various synthesis methods and properties of nanocomposites, one has to consider elementary consequences of the small size of nanoparticles. Nanoparticles are, by definition, particles with diameters below the micron dimension: generally, below 0.1 m (100 nm). A more stringent definition considers nanoparticles as particles with properties depending directly on their size. Examples are optical, electrical, or magnetic properties. Therefore, in many cases the latter definition restricts nanoparticles to particles with sizes below 1020 nm. Additionally, with decreasing particle size, the ratio of surface/volume increases, so that surface properties become crucial. The dependency of surface/volume ratio is a function of size. In this context, it is important to realize that e.g., 5 nm particles consist of only a few 1000 atoms or unit cells and possess approximately 40% of their atoms at the surface. In contrast, 0.1 m particles contain some 107 atoms or unit cells, and only 1% of their atoms are located at the surface. Therefore, the smaller the particles are, the more important will be surface properties, influencing interfacial properties, agglomeration behavior, and also - as will be shown later - physical properties of the particles. As the surface area of nanoparticles is some 100 m2/g, contaminations stemming from the various synthesis processes, as e.g., remaining precursor residuals, or solvents, may additionally influence the surface properties.
A very demonstrative example of the influence of surface area, adapted from , is to visualize a 50 kg piece of quartz (SiO2) in the form of a cube. This cube has a total edge length of about 27 cm. As a single crystal, this piece of quartz would have a total surface area of about 0.44 m2. Reducing the edge length of the contributing cubes (corresponding to crystal size) to 1 mm, the quartz cube would consist of approximately 2 107 small cubes with a total surface area of approximately 120 m2. A further reduction to 5 nm would lead to approximately 1.6 1023 very small cubes with a total surface area of around 2 km2. This is shown schematically in Figure 1.
Materials 2010, 3
Figure 1. Schematic representation of the increasing surface area while decreasing particle size, using a 50 kg quartz cube. The cubes are not true to scale.
Such extremely small particles possess only poor compacting properties. The powder density is very low, so that 100 mg of a nanopowder may take a volume of around 1 cm3. In the ideal case, assuming monomodal spherical nanoparticles, no friction between the particles, no van-der-Waals forces between the particles, no agglomeration, and a cubic face centered arrangement of particles; a maximum filling degree of 74 vol % can be obtained for a composite. In reality, the filling degree will always be significantly lower.
In addition to the established main material classes of metals, ceramics and polymers, composites, especially polymer-matrix composites (PMC), allow for a physical property tailoring using different type of fillers [7,8]. Depending on the particle size, particle shape, specific surface area and chemical nature, the following polymer matrix properties can be modified:
electrical and thermal conductivity polymer phase behavior and thermal stability mechanical properties like stiffness, Youngs modulus, wear, fatigue, and others flame retardancy  density physical properties such as magnetic, optic, or dielectric properties.
In principle, the whole bandwidth of polymer processing technology can be used for shaping, molding or replication of the polymer-based composites enabling a low cost fabrication of components and devices. On the one hand new potential applications can be realized using nanoparticles with small sizes, but on the other hand they complicate the realization of homogeneous and highly filled composites. Comprehensive books and reviews covering polymer matrix composites containing different kinds of nanosized fillers like clay, carbon nanotubes, and others, can be found in [9-11].
Depending on the synthesis conditions and the surface chemistry, the nanoparticles tend to form soft or hard agglomerates. Hard agglomerates consist of smaller particles which are connected to each other by sinter necks. They can be destroyed only by high energy milling. Soft agglomerates are accumulations of isolated particles which are connected to each other by attractive physical interactions like van-der-Waals or hydrogen bridge forces. Soft agglomerates can be disrupted into smaller particles by shear forces generating mechanical stress gradients. The interparticle interactions
Materials 2010, 3
depend mainly on the particles surface chemistry, the shape, aspect ratio and dimensionality, the interparticle distance and the polydispersity .
2. Special Features of Nanoparticles
2.1. Particle size dependent properties of inorganic nanoparticles
Ensembles of isolated nanoparticles with particle sizes below around 20 nm exhibit physical properties that may differ from their bulk counterparts. The effects are sometimes crucial, as they will strongly influence the desired or expected property of the nanocomposite. A significant influence of particle size is observed as well as on magnetic, dielectric, electronic, optical, thermodynamic, and thermomechanical, and on structural properties. The following explanations rely on general features, found in metallic, ceramic and semiconducting nanoparticles.
Size-dependent magnetic properties have been studied for around two decades. Tang et al. [13,14] reported an increasing saturation magnetization in the particle size range from 7.5 nm to 25 nm. In this size regime, the authors also observed a decrease of the transition temperature. Han et al. described similar behavior for Co-containing ferrite nanoparticles . The size dependence of saturation magnetization is depicted exemplarily in Figure 2 (left). These dependencies can be stated as general rules as nanoparticles are typically covered by a 0.5 to 1 nm thin, nonmagnetic surface layer. As the amount of surface increases with decreasing particle size, the ratio of nonmagnetic surface layer to magnetic material also increases.
Figure 2. Examples for typical particle size-dependent physical properties. Left: Saturation magnetization as a function of particle size. Data taken from . Right: Band gap energy for SnO2 as a function of particle size. Data taken from .
Size-dependent refractive indices were reported for narrow band-gap semiconducting nanoparticles
such as PbS by Kyprianidou-Leodidou et al. . Above 25 nm particle size the refractive index of PbS at different wavelengths was more or less independent of the